 Nano Express
 Open Access
 Published:
Roundrobin test on thermal conductivity measurement of ZnO nanofluids and comparison of experimental results with theoretical bounds
Nanoscale Research Letters volume 6, Article number: 258 (2011)
Abstract
Ethylene glycol (EG)based zinc oxide (ZnO) nanofluids containing no surfactant have been manufactured by onestep pulsed wire evaporation (PWE) method. Roundrobin tests on thermal conductivity measurements of three samples of EGbased ZnO nanofluids have been conducted by five participating labs, four using accurate measurement apparatuses developed in house and one using a commercial device. The results have been compared with several theoretical bounds on the effective thermal conductivity of heterogeneous systems. This study convincingly demonstrates that the large enhancements in the thermal conductivities of EGbased ZnO nanofluids tested are beyond the lower and upper bounds calculated using the models of the Maxwell and Nan et al. with and without the interfacial thermal resistance.
Introduction
Nanofluids, a new class of fluids engineered by uniformly dispersing nanostructures such as nanoparticles, nanotubes, nanorods, and nanofibers, in base fluids, have heat and mass transport properties that are far superior to those of the base fluids. For example, a number of research groups presented surprising experimental findings that nanofluids significantly enhance thermal conductivities [1–8], convective heat transfer coefficient [9–13], and heat absorption rate [14]. Therefore, these novel nanofluids have the potential to become nextgeneration coolants and working fluids for innovative applications in industries such as energy, bio and pharmaceutical industry, and chemical, electronic, environmental, material, medical and thermal engineering among others [15, 16]. Nanofluids have thus attracted considerable interest worldwide. Hundreds of research groups, in both academia and industry, are exploring nanofluids. Most recently, the European Commission launched Nanohex [17], the world's largest collaborative project for the research and development of nanofluid coolants, bringing together 12 partners from academia and industry, ranging from small and mediumsized enterprises (SMEs) to global companies such as Siemens and Thermacore.
Of all the properties of nanofluids, thermal conductivity has sparked the most excitement and controversy. The anomalous enhancement of measured thermal conductivity [1–8], as compared with the predictions of the classical models, has generated excitement in both academia and industry. However, these data became controversial years later when no anomalous enhancement in thermal conductivity was observed [18–20]. These contradictory data have generated another controversy regarding the mechanisms of enhanced thermal conductivity in nanofluids. For example, a number of investigators proposed that new mechanisms are needed to explain anomalous enhancement [21–26]. However, some others [27–29] show that the thermal conductance mechanism in nanofluids is no different from that in binary solid composites or liquid mixtures, and that thermal conductivity data lie between the wellknown effective medium bounds of the Hashin and Shtrikman (HS) [30]. But, Murshed [31] pointed out that more systematic and careful investigations are needed to resolve the controversy over the mechanism of the enhanced thermal properties. Moreover, Schmidt et al. [32] showed that the thermal conductivity of nanofluids is greater than the HamiltonCrosser model [33].
These contradictory thermal conductivity data highlight the need for more controlled synthesis and accurate characterization of nanofluids. One way to reduce data inconsistencies due to differences in sample quality, such as particle size and size distribution including agglomeration, is to conduct roundrobin tests using identical test samples. Recently, Buongiorno et al. [34] launched an International Nanofluid Property Benchmark Exercise (INPBE) to resolve the inconsistencies in the database. They reported that the nanofluids tested in INPBE exhibit thermal conductivity in good agreement with the predictions of the effective medium theory for welldispersed nanoparticles.
There are several reasons for the good agreement. First, the nanofluids used in the INPBE were manufactured by twostep method with surfactant (Set 1) and chemical reduction method with several electrolytes (Set 2) or commercial products with various surfactants and electrolytes (Sets 3 and 4). Second, measurement uncertainty analysis is essential because the measured thermal conductivity data may have biases and random variation. However, most organizations using transient hot wire method (THWM) for measurement of the thermal conductivity did not perform the measurement uncertainty analysis.
So we thought that it would be interesting to produce nanofluids by a onestep physical method with no surfactant, perform measurement uncertainty analysis, and measure the thermal conductivity of the nanofluids using very accurate thermal conductivity apparatuses.
The objectives of this study are to conduct a roundrobin test on thermal conductivity measurements of three samples of EGbased ZnO nanofluids and compare the experimental results with theoretical bounds on the effective thermal conductivity of heterogeneous systems.
Different methods of sample preparation or even small differences in the sample preparation process can cause large differences in sample properties. Therefore, in this study, one laboratory synthesized all three samples of ZnO nanofluids using onestep pulsed wire evaporation (PWE) process to be described in "Synthesis of ZnO nanofluids" section. The roundrobin exercise involved five testlaboratories that have extensive experience in the thermal conductivity measurement of nanofluids. Each participant received identical samples of ZnO nanofluids and was asked to conduct the test within 2 weeks of receipt of samples. The five participating laboratories measured the thermal conductivity of the samples of ZnO nanofluids over a temperature range from 20 to 90°C using the THWM. The results were collected, analyzed, and plotted for comparison with several theoretical bounds [30, 35, 36] on the effective thermal conductivity of heterogeneous systems.
Based on the results of these roundrobin tests using identical test samples synthesized by onestep PWE method and accurate thermal conductivity apparatus with measurement uncertainty <1.5%, we clearly show that the large enhancements in the thermal conductivity of the EGbased ZnO nanofluids are beyond the lower and upper bounds of both the Maxwell model [35] with and without the interfacial thermal resistance and the Nan et al. model [36].
Experiments
Synthesis of ZnO nanofluids
Various synthesis procedures have been used for production of nanofluids. The PWE method is one approach to fabricate nanoparticles [37]. In this study we used the PWE method mainly because the process is simple to use, and it is not time consuming to produce nanofluids samples in enough quantity for the roundrobin measurements.
Although the thermal conductivity of suspensions of ZnO nanoparticles in water or EG was studied, the previous studies [38–44] used nanofluids manufactured by the twostep method or commercial products with surfactants, as shown in Table 1. However, in this study, the EGbased ZnO nanofluids are manufactured by a onestep physical method using PWE [37] and do not contain any surfactant. Therefore, the ZnO nanofluids studied in this work are different from the previously studied ZnO nanofluids [38–44].
As shown in Figure 1, the PWE system for synthesis of EGbased ZnO nanofluids consists of three main components which are the pulsed power generator, the control panel, and the evaporation chamber with continuous wire feeding and fluid nozzle subsystems. Pure Zn wire of 99.9% with a diameter of 0.5 mm was used as a starting material and the feeding length of the wire into the reaction chamber was 100 mm. When a pulsed high voltage of 25 kV is driven through a thin wire, nonequilibrium overheating induced in the wire makes the wire evaporate into plasma within several microseconds. Then the hightemperature plasma is cooled by an interaction with an argonoxygen mixed gas, and evaporated Zn gas is condensed into smallsized particles and spontaneously immersed into EGstained chamber. The Ar:O_{2} atmosphere in the evaporation chamber facilitates formation of the zinc oxide phase. More details of the PWE method and system are given in [45].
Using the onestep PWE process, three test samples were produced: EGbased ZnO nanofluids with nanoparticle concentrations of 1.0, 3.0, and 5.5 vol.%. A transmission electron microscopy (TEM) image of ZnO nanoparticles with an average diameter of 70 nm is shown in Figure 2.
Thermal conductivity measurements and uncertainty analysis
In this study, four of the labs used a THWM developed in house to measure the thermal conductivity of EGbased ZnO nanofluids, and one of the five labs performed the thermal conductivity measurements using a commercial apparatus, LAMBDA (LAMBDA F5 Technology, Germany) with 1% error.
In order to obtain the accuracy of the transient hot wire apparatus, the measurement uncertainty analysis of the apparatus was performed by each laboratory as follows:
The thermal conductivity of fluids is calculated by Equation 1,
where k, q, ΔT and t are the thermal conductivity, the input power per unit length, the temperature rise of hot wire, and the measurement time, respectively. The thermal conductivity of fluids can be obtained if the input power unit length and temperature rise of hot wire are measured as a function of temperature. Therefore, the measurement uncertainty of the apparatus [46] is given by Equation 2,
where u_{ k }, u_{ q } , and u Δ_{ T }are the measurement uncertainties of thermal conductivity, the input power per unit length, and the temperature rise of the hot wire, respectively. Equation 2 shows that the measurement uncertainty of the thermal conductivity using the transient hot wire apparatus consists of the measurement uncertainties of input power per unit length, q, and the temperature rise of hot wire, ΔT. Here the measurement uncertainties of q and ΔT in accordance with 95% confidence interval [47, 48] are expressed by Equation 3,
where u_{ i }, B, and t_{ λ,95% }P are the measurement uncertainty of i, bias error, and estimate of the precision error in the repeated measurement data at 95% confidence. In addition, λ is the degree of freedom given by,
where N is the data size. Using this method, the measurement uncertainty of transient hot wire apparatus manufactured by each lab was determined to be less than 1.5%. In order to verify the accuracy and the reliability of this experimental system, the thermal conductivity was experimentally measured using deionized water and EG. As shown in Figure 3, a typical THW apparatus calibration with the reference fluids demonstrates that it is possible to measure thermal conductivities with less than 1.5% error, verifying the estimated measurement uncertainty of 1.5%. In Figure 3, the hollow symbols represent the calibration data and the solid symbols are the average value of the calibration data. The solid and dashed lines represent the thermal conductivity of water and EG, respectively [49].
Results and discussion
Results of the roundrobin study and statistical treatment of data
Figure 4a, b shows the thermal conductivity enhancements for the 3.0 and 5.5 vol.% ZnO nanofluids that were measured at each of the five participating labs. The thermal conductivity enhancement is defined as (k_{eff}  k_{f})/k_{f}, where k_{eff} and k_{f} are the thermal conductivity of nanofluids and base fluids, respectively. Each data point represents the ratio of the mean of 10 measured enhancements to the thermal conductivity of base fluid. Error bars show measurement uncertainty determined by the participating labs as described in the previous section. Figure 4a, b indicates that the experimental thermal conductivity data show very little dependence on temperature in the 20 to 90°C range.
Following the statistical data analysis procedures used in the INPBE study [34], we calculated the sample averages and the standard errors for all the thermal conductivity enhancement data. In Figure 4a, b, the sample average is shown as a solid line and the standard errors of the sample mean as dotted lines. As seen in Figure 4a, b, the experimental data obtained by the five participating labs lie within a narrow band about the sample average with only a few modest outliers. The data analysis shows that the standard errors of the sample mean for the 3.0 and 5.5 vol.% ZnO nanofluids samples are ±1.24 and ±3.95%, respectively.
Figure 5 shows the thermal conductivity enhancement of EGbased ZnO nanofluids at a temperature of 23°C as a function of nanoparticle volume fraction. Each data point represents the ratio of the ensemble average of enhancements measured by the participating labs at a given volume fraction to the thermal conductivity of base fluid. The error bars show the standard deviation from the ensemble average. The ZnO nanofluids show very significant increases in thermal conductivity, with a nearly 25% increase for 5.5 vol.% ZnO nanoparticles.
Comparison of experimental results with theoretical bounds
The Hashin and Shtrikman (HS) bounds on the thermal conductivity of heterogeneous systems [30] have been used for nanofluids to show that the effective medium theory can explain the enhancement of nanofluids [27, 29]. The HS upper bound is given by Equation 5 and the HS lower bound is the classical Maxwell model as given by Equation 6. Recently, Buongiorno et al. [34] used Equation 6, the classical Maxwell model with negligible interface resistance, for the upper bound for nanofluids and Equation 7, the Maxwell model with interface resistance, for the lower bound for nanofluids.
Upper bound of Hashin and Shtrikman [30]
Upper bound of the Maxwell Model (no interfacial thermal resistance) [35]
Lower bound of the Maxwell Model (with interfacial thermal resistance) [50]
where k_{f}, k_{p}, r_{p}, R_{b}, and φ are the thermal conductivities of base fluids and nanoparticles, radius of nanoparticles, interfacial thermal resistance, and volume fraction of nanoparticles, respectively.
Figures 6 and 7 show comparisons of experimental thermal conductivity enhancements of 3.0 vol.% and 5.5 vol.% ZnO nanofluids with the three theoretical bounds of Hashin and Shtrikman and Maxwell models. The properties, such as the thermal conductivities of EG [49] and ZnO nanoparticles [51], used for calculating the theoretical bounds are summarized in Table 2. The upper bound of Hashin and Shtrikman, which was used by Eapen et al. [27] and Kelbinski et al. [29], dramatically overestimates the thermal conductivity of ZnO nanofluids. The HS upper bound corresponds to large pockets of fluid separated by linked chainforming or clustered nanoparticles [29]. The long wirelike structures made of perfectly aligned nanoparticles are not realizable with dilute nanofluids with welldispersed nanoparticles. Furthermore, it is almost impossible to separate fluid by nanoparticle chains in nanofluids, although nanoparticles can be partially aggregated in nanofluids. Therefore, the upper bound given by the HS model is not applicable to nanofluids. More realistic upper and lower bounds for nanofluids having low concentration of welldispersed nanoparticles are given by Buongiorno et al. [34]. It is clear from Figures 6 and 7 that the thermal conductivity enhancements of EGbased ZnO nanofluids are larger than the upper bound of the Maxwell model.
In addition, we used the generalized Maxwell model developed by Nan et al. [36] with and without interfacial resistance for the lower and upper bounds for nanofluids. The Nan et al. model is given in Equation 8.
Nan et al. [36] model
, , , ,
where a_{ii}, a_{k}, L_{ii}, p, φ, and are the diameter of the ellipsoid, Kapitza radius, geometrical factors dependent on the particle shape, aspect ratio of the ellipsoid, volume faction, and equivalent thermal conductivities, respectively. R_{bd} is the interfacial thermal resistance, also known as thermal boundary resistance, or Kapitza resistance.
Figures 8 and 9 show comparisons of the experimental thermal conductivity enhancements of 3.0 and 5.5 vol.% ZnO nanofluids with the theoretical bounds of Nan et al. model. The interfacial thermal resistance used for the upper bound is 0 m^{2}K/W and that for the lower bound is 10^{8} m^{2}K/W [52]. It can be seen clearly that all the thermal conductivity data lie above the bounds predicted by the model of Nan et al.
The comparisons of experimental results with theoretical models convincingly demonstrate that the large enhancements in the thermal conductivities of EGbased ZnO nanofluids are beyond the lower and upper bounds calculated using the models of Maxwell and Nan et al. with and without the interfacial thermal resistance the predictions of the effective medium theory for welldispersed nanoparticles.
Conclusions
Ethylene glycol (EG)based ZnO nanofluids containing no surfactant have been manufactured by onestep physical method using the PWE process. Roundrobin tests on thermal conductivity measurements of three samples of EGbased ZnO nanofluids have been conducted and the results have been compared with several theoretical bounds on the effective thermal conductivity of heterogeneous systems. The enhancements of the thermal conductivity of the ZnO nanofluids are beyond the upper and lower bounds of both the Maxwell model and Nan et al. model. Especially, the enhancement of the 5.5 vol.% ZnO nanofluids at 23 C is nearly 25%, while the enhancement predicted by the upper bound of the Maxwell model is at precisely 16.5%. Thus, the discrepancies in the thermal conductivity of the ZnO nanofluids tested in this study cannot be fully explained by the effective medium theory for welldispersed nanoparticles. Further research is needed to understand and resolve the controversies about contradictory data and new mechanisms of enhanced thermal conductivity in nanofluids.
Abbreviations
 EG:

ethylene glycol
 HS:

Hashin and Shtrikman
 INPBE:

International Nanofluid Property Benchmark Exercise
 PWE:

pulsed wire evaporation
 SMEs:

small and mediumsized enterprises
 TEM:

transmission electron microscopy
 THWM:

transient hot wire method
 ZnO:

zinc oxide.
References
 1.
Eastman JA, Choi SUS, Li S, Yu W, Thompson LJ: Anomalously increased effective thermal conductivities of ethylene glycolbased nanofluids containing copper nanoparticles. Appl Phys Lett 2001, 78: 718–720. 10.1063/1.1341218
 2.
Choi SUS, Zhang ZG, Yu W, Lockwood FE, Grulke EA: Anomalous thermal conductivity enhancement in nanotube suspensions. Appl Phys Lett 2001, 79: 2252–2254. 10.1063/1.1408272
 3.
Patel HE, Das SK, Sundararajan T, Nair AS, George B, Pradeep T: Thermal conductivity of naked and monolayer protected metal nanoparticles based nanofluids: manifestation of anomalous enhancement and chemical effects. Appl Phys Lett 2003, 83: 2931–2933. 10.1063/1.1602578
 4.
Das SK, Putra N, Thiesen P, Roetzel W: Temperature dependence of thermal conductivity enhancement for nanofluids. J Heat Transfer 2003, 125: 567–574. 10.1115/1.1571080
 5.
Hong KS, Hong TK, Yang HS: Thermal conductivity of Fe nanofluids depending on the cluster size of nanoparticles. Appl Phys Lett 2006, 88: 031901. 10.1063/1.2166199
 6.
Li CH, Peterson GP: Size effect on the effective thermal conductivity of Al_{2}O_{3}/Di water nanofluids. J Appl Phys 2006, 99: 084314. 10.1063/1.2191571
 7.
Chopkar M, Das PK, Manna I: Synthesis and characterization of nanofluid for advanced heat transfer applications. Scripta Mater 2006, 55: 549–552. 10.1016/j.scriptamat.2006.05.030
 8.
Jana S, SalehiKhojin A, Zhong WH: Enhancement of fluid thermal conductivity by the addition of single and hybrid nanoadditives. Thermochim Acta 2007, 462: 45–55. 10.1016/j.tca.2007.06.009
 9.
Pak BC, Cho Y: Hydrodynamic and heat transfer study of dispersed fluids with submicron metallic oxide particles. Exp Heat Transfer 1998, 11: 151–170. 10.1080/08916159808946559
 10.
Xuan Y, Li Q: Investigation on convective heat transfer and flow features of nanofluids. ASME J Heat Transfer 2003, 125: 151–155. 10.1115/1.1532008
 11.
Wen D, Ding Y: Experimental investigation into convective heat transfer of nanofluid at the entrance rejoin under laminar flow conditions. Int J Heat Mass Transfer 2004, 47: 5181–5188. 10.1016/j.ijheatmasstransfer.2004.07.012
 12.
Ding Y, Alias H, Wen D, Williams RA: Heat transfer of aqueous suspensions of carbon nanotubes (CNT nanofluids). Int J Heat Mass Transfer 2006, 49: 240–250. 10.1016/j.ijheatmasstransfer.2005.07.009
 13.
Nguyen CT, Roy G, Gauthier C, Galanis N: Heat transfer enhancement using Al_{2}O_{3}water nanofluid for an electronic liquid cooling system. Appl Therm Eng 2007, 27: 1501–1506. 10.1016/j.applthermaleng.2006.09.028
 14.
Kim JK, Jung JY, Kang YT: The effect of nanoparticles on the bubble absorption performance in a binary nanofluid. Int J Refrigeration 2006, 29: 22–29. 10.1016/j.ijrefrig.2005.08.006
 15.
Choi SUS: Nanofluids: From vision to reality through research. ASME J Heat Transfer 2009, 131: 033106. 10.1115/1.3056479
 16.
Wang L, Fan J: Nanofluids research: Key issues. Nanoscale Res Lett 2010, 5: 1241–1252. 10.1007/s1167101096386
 17.
 18.
Zhang X, Gu H, Fujii M: Effective thermal conductivity and thermal diffusivity of nanofluids containing spherical and cylindrical nanoparticles. J Appl Phys 2006, 100: 044325. 10.1063/1.2259789
 19.
Putnam SA, Cahill D, Braun PV, Ge Z, Shimmin RG: Thermal conductivity of nanoparticles suspensions. J Appl Phys 2006, 99: 084308. 10.1063/1.2189933
 20.
Timofeeva EV, Gavrilov AN, McCloskey JM, Tolmachev YV, Sprunt S, Lopatina LM, Selinger JV: Thermal conductivity and particle agglomeration in alumina nanofluids: experiment and theory. Phys Rev E 2007, 76: 061203. 10.1103/PhysRevE.76.061203
 21.
Xuan Y, Li Q, Hu W: Aggregation structure and thermal conductivity. AIChE J 2003, 49: 1038–1043. 10.1002/aic.690490420
 22.
Yu W, Choi SUS: The role of interfacial layers in the enhanced thermal conductivity of nanofluids: a renovated Maxwell model. J Nanopart Res 2003, 5: 167–171. 10.1023/A:1024438603801
 23.
Jang SP, Choi SUS: Role of Brownian motion in the enhanced thermal conductivity of nanofluids. Appl Phys Lett 2004, 84: 4316–4318. 10.1063/1.1756684
 24.
Prasher R, Bhattacharya P, Phelan PE: Thermal conductivity of nanoscale colloidal solutions (nanofluids). Phys Rev Lett 2005, 94: 025901. 10.1103/PhysRevLett.94.025901
 25.
Xuan Y, Li Q, Zhang X, Fujii M: Stochastic thermal transport of nanoparticle suspensions. J Appl Phys 2006, 100: 043507. 10.1063/1.2245203
 26.
Wang L, Wei X: Nanofluids: synthesis, heat conduction, and extension. ASME J Heat Transfer 2009, 131: 033102. 10.1115/1.3056597
 27.
Eapen J, Williams WC, Buongiorno J, Hu LW, Yip S, Rusconi R, Piazza R: Meanfield versus microconvection effects in nanofluid thermal conduction. Phys Rev Lett 2007, 99: 095901. 10.1103/PhysRevLett.99.095901
 28.
Prasher R, Evans W, Meakin P, Fish J, Phelan P, Keblinski P: Effect of aggregation on thermal conduction in colloidal nanofluids. Appl Phys Lett 2006, 89: 143119. 10.1063/1.2360229
 29.
Keblinski P, Prasher R, Eapen J: Thermal conductance of nanofluids: is the controversy over? J Nanopart Res 2008, 10: 1089–1097. 10.1007/s1105100793521
 30.
Hashin Z, Shtrikman S: A variational approach to the theory of effective magnetic permeability of multiphase materials. J Appl Phys 1962, 33: 3125–3131. 10.1063/1.1728579
 31.
Murshed SMS: Correction and comment on "thermal conductance of nanofluids: is the controversy over? J Nanopart Res 2009, 11: 511–512. 10.1007/s1105100895532
 32.
Schmidt AJ, Chiesa M, Torchinsky DH, Johnson JA, Nelson KA, Chen G: Thermal conductivity of nanoparticle suspensions in insulating media measured with a transient optical grating and a hotwire. J Appl Phys 2008, 103: 083529. 10.1063/1.2908887
 33.
Hamilton RL, Crosser OK: Thermal conductivity of heterogeneous two component systems. Ind Eng Chem Fundam 1962, 1: 187–191. 10.1021/i160003a005
 34.
Buongiorno J, et al.: A benchmark study on the thermal conductivity of nanofluids. J Appl Phys 2009, 106: 094312. 10.1063/1.3245330
 35.
Maxwell JC: A Treatise on Electricity and Magnetism. 1st edition. Oxford: Clarendon Press; 1873.
 36.
Nan CW, Birringer R, Clarke DR, Gleiter H: Effective thermal conductivity of particulate composites with interfacial thermal resistance. J Appl Phys 1997, 81: 6692–6699. 10.1063/1.365209
 37.
Wang Q, Tang H, Shi J, Zou G: Onestep synthesis of the nanometer particles of ϒ Fe_{2}O_{3}by wire electrical explosion method. Mater Res Bull 2001, 36: 503–509. 10.1016/S00255408(01)00544X
 38.
Kim SH, Choi SR, Kim D: Thermal conductivity of metaloxide nanofluids: Particle size dependence and effect of laser irradiation. J Heat Transfer 2007, 129: 298–307. 10.1115/1.2427071
 39.
Yu W, Xie H, Chen L, Li Y: Investigation of thermal conductivity and viscosity of ethylene glycol based ZnO nanofluid. Thermochim Acta 2009, 491: 92–96. 10.1016/j.tca.2009.03.007
 40.
Moosavi M, Goharshadi EK, Youssefi A: Fabrication, characterization, and measurement of some physicochemical properties of ZnO nanofluids. Int J Heat Fluid Flow 2010, 31: 599–605. 10.1016/j.ijheatfluidflow.2010.01.011
 41.
Raykar VS, Singh AK: Thermal and rheological behavior of acetylacetone stabilized ZnO nanofluids. Thermochim Acta 2010, 502: 60–65. 10.1016/j.tca.2010.02.007
 42.
Shen B: Minimum quantity lubrication grinding using nanofluids. In Doctoral thesis. University of Michigan; 2008.
 43.
Vajjha RS, Das DK: Measurement of thermal conductivity of three nanofluids and development of new correlations. Int J Heat Mass Transfer 2009, 52: 4675–4682. 10.1016/j.ijheatmasstransfer.2009.06.027
 44.
Xie H, Li Y, Yu W: Intriguingly high convective heat transfer enhancement of nanofluid coolants in laminar flows. Phys Lett A 2010, 374: 2566–2568. 10.1016/j.physleta.2010.04.026
 45.
Uhm YR, Kim WW, Kim SJ, Kim CS, Rhee CK: Magnetic nanoparticles of Fe_{2}O_{3}synthesized by the pulsed wire evaporation method. J Appl Phys 2003, 93: 7196–7198. 10.1063/1.1558234
 46.
Abernethy RB, Benedict RP, Dowdell RB: ASME Measurement Uncertainty. ASME J Fluids Eng 1985, 107: 161–164. 10.1115/1.3242450
 47.
Richard SF, Donald EB: Theory and Design for Mechanical Measurements. 2nd edition. New York: Wiley; 1995.
 48.
Kim SJ, Jang SP: Experimental and numerical analysis of heat transfer phenomena in a sensor tube of a mass flow controller. Int J Heat Mass Transfer 2001, 44: 1711–1724. 10.1016/S00179310(00)002167
 49.
Incropera FP, Dewitt DP, Bergman TL, Lavine AS: Fundamentals of Heat and Mass Transfer. 6th edition. New York: Wiley; 2007.
 50.
Hasselman DPH, Johnson LF: Effective thermal conductivity of composites with interfacial thermal barrier resistant. J Comp Mater 1987, 21: 508–515. 10.1177/002199838702100602
 51.
Touloukian YS: Thermophysical Properties of Matter. 2nd edition. New York: IFI/Plenum; 1970.
 52.
Prasher R, Bhattacharya P, Phelan PE: Brownianmotionbased convectiveconductive model for the thermal conductivity of nanofluids. J Heat Transfer 2006, 128: 588–595. 10.1115/1.2188509
Acknowledgements
This work was supported by Energy and Resources Technology R&D Program (2008ECM 11P080000) under the Ministry of Knowledge Economy, Republic of Korea. We thank the participants in the roundrobin study for their substantial investments of both time and resources. This work could not have been accomplished without their passion and efforts.
Author information
Additional information
Competing interests
The authors declare that they have no competing interests.
Authors' contributions
WHL, CKR, LK, JL, SPJ and SC conceived of the study and participated in its design and coordination. KWL, HYB, GJL, CKK, SWH, YK, DK, SHK, KSH, HJK, HJH, and SHL carried out the experiments. SPJ performed the statistical analysis. SPJ and GJL drafted the manuscript. CJC and JHL checked the equations, figures, and references. SC guided the program and revised the manuscript. All authors read and approved the final manuscript.
Authors’ original submitted files for images
Below are the links to the authors’ original submitted files for images.
Rights and permissions
About this article
Cite this article
Lee, W., Rhee, C., Koo, J. et al. Roundrobin test on thermal conductivity measurement of ZnO nanofluids and comparison of experimental results with theoretical bounds. Nanoscale Res Lett 6, 258 (2011) doi:10.1186/1556276X6258
Received
Accepted
Published
DOI
Keywords
 Thermal Conductivity
 Effective Thermal Conductivity
 Base Fluid
 Maxwell Model
 Thermal Conductivity Measurement